- Nano Express
- Open Access
Fabrication of Poly(acrylic acid)/Boron Nitride Composite Hydrogels with Excellent Mechanical Properties and Rapid Self-Healing Through Hierarchically Physical Interactions
Nanoscale Research Letters volume 13, Article number: 393 (2018)
Many living tissues possess excellent mechanical properties and self-healing ability. To mimic these living tissues, a series of novel composite hydrogels, poly(acrylic acid)/surface-modified boron nitride nanosheets (PAA/BNNS-NH2) were fabricated simply through hierarchically physical interactions: molecular-scale metal coordination interaction between –COOH of PAA and Fe3+ and nanoscale H-bond between –COOH of PAA and –NH2 of BNNS-NH2. The composite hydrogels exhibit both excellent mechanical properties (including enhanced fracture stress, elongation, toughness, Young’s modulus, and dissipated energy) and rapid healing ability without any external stimulus. Especially, the B0.5P70 (the hydrogel with BNNS concentration of 0.5 mg mL− 1, the water content of 70 wt%) exhibits a fracture stress of ~ 1311 kPa and toughness of ~ 4.7 MJ m− 3, almost ~ 3 times and ~ 8 times to B0P70, respectively. The excellent properties, combined with the simple preparation method, endow these composite hydrogels with potential applications.
Hydrogels with three-dimensional networks formed by covalent bonds and/or physical interactions crosslinking containing a large amount of water possess high hydrophilicity, water-holding capacity and unexceptional biocompatibility [1,2,3,4], enabling to be one of the most popular biomaterials. However, most hydrogels have poor mechanical property, which largely limited the applications. It is well known that many living tissues, such as muscle, ligament, and skin, possess excellent mechanical property and significant ability to heal wounds autonomously [5,6,7]. Inspired by these living tissues, materials with high mechanical properties and self-healing ability have been explored for various applications [8, 9], including tissue engineering, drug release, wound dressing, contact lenses, sensors, and actuators [2, 10,11,12]. Ihsan et al. reported a polyampholyte hydrogel self-healed through re-forming the ironic bonds at fracture surface . Zhang et al. designed a PVA self-healable hydrogel with fast self-healing process through hydrogen bonds . Tao et al. prepared a cold resistance self-healing hydrogel crosslinked by dynamic catechol-borate ester bonding which enable to self-heal at both room temperature and low temperature . However, all these self-healable materials have a common weakness: poor mechanical property [15,16,17,18,19] largely limited the applications.
In order to improve the mechanical property of the hydrogels, some inorganic nanomaterials have been introduced to the crosslinked systems. Han et al. reported a supermolecular hydrogel by using graphene oxide nanosheets to reduce the temperature for self-healing . Si et al. exploited a new ultrahigh-water-content, super-elastic, and shape-memory nanofiber-assembled hydrogels . The flexible SiO2 nanofibers were introduced to enhance mechanical property and to accelerate shape memory and pressure response. Especially, Duan et al. developed poly(vinyl alcohol)/boron nitride nanosheet (PVA/BNNS) composite hydrogels with enhanced mechanical properties . Gao et al. fabricated a nanocomposite hydrogel filled with exfoliated montmorillonite which dramatically improved the fracture elongation . Zhong et al. designed graphene oxide (GO)/poly(acrylic acid) (PAA/GO) nanocomposite hydrogels which significantly enhanced the mechanical properties . Novel composite self-healing hydrogels with enhanced mechanical property are still highly pursued although exploited hydrogels have advanced significantly in recent years. Boron nitride nanosheets, “white graphene”, exhibit many excellent properties including superb mechanical properties, extraordinary chemical inertness, and remarkable non-toxicity [24,25,26]. Notably, surface-modified BN nanosheets served as nanofillers in the nanocomposite hydrogels enhance mechanical and thermal properties and have been reported in recent works [27, 28]. Therefore, the development of a novel composite hydrogel with surface-modified BN nanosheets is still highly pursued.
Here, the novel composite hydrogels are fabricated from poly(acrylic acid) (PAA) and amino groups surface-modified boron nitride nanosheet (BNNS-NH2) through hierarchically physical interactions: molecular-scale metal coordination interaction between –COOH of PAA and ferric ion (Fe3+) and nanoscale H-bond between –COOH and BNNS-NH2 were reported. The introduction of BNNS-NH2 enhanced the mechanical property and accelerated self-healing process of the hydrogels. This work provides a new route to prepare hydrogels with excellent mechanical properties and rapid self-healing ability.
Potassium persulfate (KPS; 99.0%) and FeCl3·6H2O (99.0%) were purchased from J&K Chemical Technology, and acrylic acid (AA; 98.0%) was purchased from Sigma-Aldrich. All these chemicals were used as received without any purification. Rhodamine B (95.0%) was purchased from Sigma-Aldrich. BNNS-NH2 was obtained by our previous work . Deionized water was used throughout the experiments.
Preparation of BNNS-NH2 Dispersion
BNNS-NH2 was prepared according to our previous work . In order to make BNNS-NH2 steadily dispersed in the polymer network, it is indispensable to prepare the BNNS-NH2 water dispersions. To obtain the stable BNNS-NH2 dispersions, magnetic stirring and ultrasound bath were utilized at room temperature. The BNNS-NH2 dispersions with concentration of 1.0, 0.8, 0.5, and 0.1 mg mL− 1 were obtained by the following procedure. The 100 mg, 80 mg, 50 mg, and 10 mg of BNNS-NH2 were added in 100 mL of deionized water, respectively, under magnetic stirring (1000 rpm) for 24 h at room temperature in air ambient to obtain mixtures, and then the mixtures were sonicated (20 kHz) at room temperature for 2 h in air ambient to get stable dispersions. For prohibiting loss of the water solution, the obtained dispersions were preserved in sealed vessels with different marks for following preparation of self-healing hydrogels.
Preparation of Self-Healing Hydrogel
PAA as the common polymer with abundant –COOH groups enables to establish the amount of intrachain and interchain hydrogen bonds which endow the polymer to possess superior elasticity and favorable strength . In addition, metal coordination interactions are set up between –COOH of PAA and ferric ion (Fe3+). The two kinds of reversible non-covalent bonds equipped the hydrogel with self-healing property. The hydrogels crosslinked by non-covalent bonds always possess inferior mechanical properties. In order to enhance the strength of the hydrogel, BNNS-NH2 was introduced to the polymer three-dimensional network, which established hydrogen bonds between –NH2 of BNNS-NH2 and –COOH of PAA. Here, the composite PAA/BNNS-NH2 hydrogels were abbreviated as BxPy, in which B represents BNNS-NH2, x is the content of the BNNS-NH2 (mg mL− 1), P means PAA/BNNS-NH2 composite hydrogel, and y refers to the water content of the PAA/BNNS-NH2 composite hydrogel (mass fraction, wt%). The hydrogels were prepared according to a procedure described below. Typically, 10 mL of AA, 0.25 g of FeCl3·6H2O (1.05 mol% of AA), and 0.1 g of KPS (0.25 mol% of AA) were dissolved in BNNS-NH2 dispersions with different concentrations or deionized water under magnetic stirring (1000 rpm) at room temperature for 10 min under air ambient to form a homogeneous mixture. After that, N2 was bubbled into the mixture to remove oxygen (10 min), and then polymerization was carried out at 25 °C in water bath for 6 h to form hydrogels. Hydrogels prepared as aforementioned procedure and parameters from BNNS-NH2 dispersions with the concentration of 1.0, 0.8, 0.5, and 0.1 mg mL− 1 were denoted as B1P90, B0.8P90, B0.5P90, and B0.1P90, respectively, while hydrogels prepared from deionized water was named as B0P90.
It is well known that the hydrogels with different water contents possess entirely different mechanical properties. In order to characterize the influence of water content to the mechanical properties of the hydrogels, the hydrogels with different water contents were prepared as follows. Firstly, the BxP90 hydrogels were prepared as the aforementioned procedure and parameters. Then, the as-prepared BxP90 hydrogels were exposed in air at room temperature for different times depending on the final water content of the hydrogels. Thereinto, the obtained drying hydrogels with different water contents were labeled as BxP70, BxP50, and BxP25, respectively. The water content was calculated by the formula: water content = Ww/Wt, where the Ww is the weight of the water and Wt is the whole weight of the hydrogel. On the other hand, the crosslinking densities of BxP90 hydrogels were calculated from the results of rheological measurements, and it is well known that the higher crosslinking density leads to the more robust mechanical property. To verify the theory, it is indispensable to carry out the tensile tests. However, the BxP90 hydrogels were so soft that the electrical universal material testing machine cannot recognize the sample exhibiting no load, so the composite hydrogels with lower water content were highly required to fabricate. The hydrogels with different water contents were cut into different shapes or sizes for the following various tests.
In order to characterize the mechanical properties of the hydrogels, the as-prepared hydrogels were cut into a flaky shape (50 mm × 2 mm × 2 mm) and tested by the electrical universal material testing machine with a 200 N load cell under a speed of 50 mm min− 1 at 25 °C and a humidity of approximately 45%. The tensile stress (σ) representing strength was calculated by the equation: σ = F/(a × b), where F, a, and b were force of loading and width and thickness of hydrogels, respectively. The strain (ε) representing stretchability was defined as the change of the length, illustrated by the formula: ε = (l − l0)/l0 × 100%, where l and l0 represent the lengths after and before testing, respectively. Stiffness was characterized by Young’s modulus which was obtained from the slope of the stress-strain curve at the low strains. The toughness of the samples was illustrated as the area under stress-strain curves. The cyclic tensile tests were performed at the same experimental condition which aimed to obtain the dissipated energy. The dissipated energy was characterized by the area between the loading-unloading curves and X-axis.
The Fourier-transform infrared (FTIR) spectra was carried out to record the samples’ FTIR characters, which were recorded on a Thermo Scientific Nicolet 6700 spectrometer in attenuated total reflection (ATR) mode, with a resolution of 4 cm− 1 within the range 400–4000 cm− 1. The morphology of the hydrogels after the frozen drying process was observed on scanning electronic micrographs (SEM, Carl Zeiss AG, ZEISS EV0 MA15). In order to analyze the viscoelasticity of the hydrogels and calculate the crosslinking density, the rheological measurements were carried out by using a rheometer (HAAKE MARS III Thermo Fisher Scientific Limited, China) to measure the storage moduli (G’) and loss moduli (G”). The tensile tests were carried out to analyze the mechanical properties of the samples, which were conducted using an electrical universal material testing machine with a 200 N load cell (Instron 2360).
Results and Discussion
The PAA/BNNS-NH2 composite hydrogels were simply formed by in situ polymerization of AA, with the presence of Fe3+ and the BNNS-NH2. The as-formed PAA macromolecular chains were crosslinked by hierarchically physical interactions: metal coordination interaction between carboxyls (–COOH) of the PAA and Fe3+ in molecular scale, and hydrogen bond interaction between –COOH of the PAA and –NH2 of BNNS-NH2 in nanoscale, resulting in the formation of three-dimensional networks (Scheme 1).
The two different types of physical interactions within the PAA/BNNS-NH2 composite hydrogels were revealed by FTIR spectroscopy firstly. From the results in Fig. 1, PAA shows a characteristic stretching (–C=O stretching) at 1690 cm− 1, which has shifted to 1620 cm− 1 in the PAA/BNNS-NH2 composite hydrogel. This shift indicates the existence of hydrogen bond interactions between –COOH of PAA and –NH2 of BNNS-NH2 [30, 31]. The presence of hydrogen bond can be verified by the fact that the characteristic peaks at 3400 cm− 1for –COOH became less obvious in the composite hydrogel [32, 33]. The peak at 3230 cm− 1 can be assigned to N–H stretching vibration in the composite hydrogel. Metal coordination interaction was revealed by the peak at 620 cm− 1 in both PAA hydrogel and composite hydrogel, demonstrating that metal coordination interaction between Fe3+ and –COO− was formed in the network system . The in-plane B–N stretching at 1388 cm− 1 and the out-of-plane B-N-B bending vibrations at 1780 cm−1can be seen from composite hydrogel (Fig. 1a), confirming the presence of BNNS-NH2.
After drying, the morphologies of these hydrogels were observed by SEM. Porous structures have been observed in PAA hydrogel (Fig. 2a, b) and BxPy composite hydrogel (Fig. 2c). The larger pores have an average diameter of around dozens of micrometers and the smaller pores have an average diameter in nanoscale. The presence of pores might provide high stretchability and squeezability to the hydrogels . Compared to PAA hydrogels, the pores within the composite hydrogel are more isolated and uniform in sizes (Fig. 2c). And the BNNSs-NH2 can be observed in a SEM image (Fig. 2d) of hydrogel containing BNNSs-NH2 and were pointed out by arrows, and the insert image further verified the presence of the BNNS-NH2 . To understand the effects of the two-type interactions, tensile tests of composite hydrogels with different BNNS-NH2 concentrations were conducted, and results from these hydrogels with different water contents are shown in Fig. 3a–c. Without BNNS-NH2, the fracture stress of B0P70 hydrogel was about 406 kPa, and the facture stress of B0.1P70 increased to 526 kPa by introducing a small amount of BNNS-NH2. The B0.5P70 exhibits a fracture stress of 1311 kPa, almost three times to B0P70 and two times to B0.1P70, as shown in Fig. 3a. The result far exceeded previous composite hydrogels in published work . This means that the hydrogen bond formed between –COOH of PAA and –NH2 of BNNS-NH2 significantly enhanced the mechanical properties . However, the fracture stress decreased when the BNNS-NH2 concentration continued to increase. The fracture stress becomes even lower than that of B0P70, which indicated that a prime balance of metal coordination interactions and hydrogen bonds was achieved at the BNNS-NH2 concentration of 0.5 mg mL− 1. Correspondingly, the greatest fracture stresses were also realized at the same BNNS-NH2 concentration (0.5 mg mL− 1) within composite hydrogels with the water content of 50 wt% and 25 wt% (Fig. 3b, c) which was an important factor to affect the mechanical properties of the hydrogel [37, 38]. The fracture stresses of the composite hydrogels were remarkably improved (Additional file 1: Figure S1-S5) when water content decreased to 50 wt% and to 25 wt%, attributed to the narrow space between chains at low water content . Notably, the BxPy hydrogels were able to withstand tensile, knotting, bending, and torsion even under high degree of deformations (Fig. 3d–g, Additional file 1: Figure S6). The addition of BNNS-NH2 might slightly change the pH of the solution due to the presence of –NH2 groups, leading to a change in association constant between –COOH and Fe3+. The balance between metal coordination interactions and hydrogen bonds was dependent on the BNNS-NH2 concentration with the constant content of Fe3+. The excellent mechanical behaviors of the composite hydrogel stemmed from the optimum balance between the metal coordination interaction in molecular scale and the hydrogen bond interactions in nanoscale .
The effects of BNNS-NH2 concentration on mechanical properties of BxP90 were studied by rheological measurement (Fig. 4a). For all the samples, their storage moduli (G’) are always higher than the corresponding loss moduli (G”) in the frequency range from 0.1 to 100 rad s− 1, indicating the formation of three-dimensional networks [34, 36]. With the increase of frequency, both G’ and G” increased, but the increase in G” is more sharp, showing their shear-thin behaviors . B0.5P90 exhibited the highest G’, which is consistent with the results from the tensile tests. From the equilibrium shear modulus (Ge), crosslinking density (N) of these hydrogels can be calculated by using formula 1 [39,40,41].
Here, Ge, R, and T are the terrace value of G’, gas constant, and absolute temperature, respectively. The crosslinking density is shown in Fig. 4b. With increase in the concentration of BNNS-NH2, the crosslinking density increased, which demonstrates that BNNS-NH2 also served as a crosslinker in the composite hydrogels through hydrogen bond interactions between –COOH of PAA and –NH2 of BNNS-NH2. However, the crosslinking density decreased when the BNNS-NH2 concentration is over 0.5 mg mL− 1 which corresponded with the results of the mechanical properties . It is illustrated that the excess BNNS-NH2 leads to reunion of the nanosheets which impairs the enhancement to the composite hydrogels such as B0.8Py and B1.0Py [41, 42].
To obtain hydrogels with excellent mechanical properties, the optimal balance of hydrogen bond interactions and metal coordination interactions can be achieved by adjusting the BNNS-NH2 concentrations while the content of Fe3+ is constant. Toughness and Young’s modulus representing stiffness are shown in Fig. 5a and Fig. 5b, respectively [24, 36, 37]. From Fig. 5a, hydrogels became stiff with decreasing water content or increasing BNNS-NH2 concentration till 0.5 mg mL− 1 consistent with the results of tensile test (Additional file 1: Figure S7).
The toughness is observed in Fig. 5b. It is clear that toughness increases with decreasing water content, similar to the trend of Young’s modulus. Without BNNS-NH2, the toughness of B0P70 was about ~ 0.5 MJ m− 3, and with BNNS-NH2, the toughness of B0.5P70 increased to ~ 4.7 MJ m− 3, almost eight times to that of B0P70. The B0.5P25 exhibited the highest Young’s modulus of ~ 17.9 MPa, highest tensile strength of ~ 8491 kPa, and highest toughness of ~ 10.5 MJ m− 3, which is far higher than that of B0P25.
The stiffness of most polymer hydrogels decreases with increase in the corresponding toughness. According to the Lake-Thomas model [42, 43], toughness increases but stiffness decreases with decreasing crosslinking density. In this work, a novel type hydrogel with both high stiffness and high toughness (B0.5Py) (Fig. 5) has been fabricated, which is different from the conventional hydrogels (high stiffness/low toughness or low stiffness/high toughness). The exceptional properties can be ascribed to the existence of hierarchical interactions: metal coordination interactions in molecular scale and hydrogen bonds in nanoscale.
Cyclic tensile tests of BxP70 and BxP50 were conducted at the strain of 200% (Fig. 6a, b). Obvious hysteresis loops were observed for BxP70 and BxP50, and BxP50 showed much larger hysteresis loops, indicating the water content determining energy dissipation owing to more hydrogen bonds being established between polymer chains because of the shrunken networks . The dissipated energy increased with increasing BNNS-NH2 concentration, and the maximum value was obtained at the concentration of 0.5 mg mL− 1 due to the establishment of numerous hydrogen bonds between BNNS-NH2 and PAA chains . However, the dissipated energy decreased when BNNS-NH2 concentration increased to 0.8 and to 1.0 mg mL− 1, owing to the high concentration of BNNS-NH2 leading to aggregation of the nanosheets [41, 42]. This explanation is also suitable for specific stress-strain curves and rheology results of the BxPy hydrogels.
The rapid self-healing process can be realized without any external stimulus based on the abundant physical interactions: metal coordination interactions and hydrogen bonds. As shown in Fig. 7a–c, the original hydrogel was cut to three parts (two parts were dye to red by Rhodamine B to distinguish the scars of the damaged hydrogel) and then they were contacted at the damaged surfaces. Without any external stimulus, the cut hydrogel contacted for 10 min at room temperature, the healed hydrogel can be stretched to certain strain. Self-healing efficiency can be calculated from the ratio of fracture stress of the healed hydrogels and the original hydrogels. Original B0P70 exhibited fracture stress of ~ 410 kPa, and the corresponding healed hydrogel exhibited a fracture stress of only ~ 37 kPa, indicating that the self-healing efficiency was only 9%. In comparison, the fracture stress of original and healed B1P70 were about ~ 203 kPa and ~ 166 kPa, respectively, and the self-healing efficiency is about 81%, which is significantly higher than the hydrogels without the BNNS-NH2. Similarly, as shown in Fig. 7e, the self-healing efficiency of B0P50 hydrogel was 31.8%, while the B1P50 hydrogel was 94.6%. This result indicates that the presence of nanoscale hydrogen bonds between BNNS-NH2 and PAA polymer chains in nanoscale enhanced the self-healing ability ascribing that the content of reversible bonds is the key influencing factor of the self-healing efficiency, and it is well known that the self-healing efficiency is proportional to the content of the reversible bonds [16, 21, 36, 42]. However, while the water content was reduced to 25 wt% (Additional file 1: Figure S8), the self-healing efficiency declined sharply, because the movement of Fe3+ was impeded at such a low water content. This assumption was confirmed by the fact that healing efficiency of BxP90 was much better than other water content, with only 10 min required attributed to the reason that higher water contents make the Fe3+ to migrate easily and re-establish hydrogen bonds readily .
In summary, the novel composite hydrogels have been fabricated through hierarchically physical interactions: the metal coordination interaction in molecular scale and hydrogen bond in nanoscale. The hydrogels exhibit enhanced stiffness (about 17.9 MPa), toughness (about 10.5 MJ m− 3), extension, and self-healing ability. The reversibility of metal coordination interaction and hydrogen bond interaction is responsible for the enhanced mechanical properties and self-healing efficiency. Combined with facile preparation, enhanced mechanical properties and self-healing ability make these composite hydrogels suitable for many potential applications.
- BxPy :
Composite hydrogel with the BNNS-NH2 concentration of x mg mL− 1 and water content of y wt%
- Fe3+ :
- PAA/BNNS-NH2 :
Poly(acrylic acid)/surface-modified boron nitride nanosheets
Graphene oxide/poly(acrylic acid)
Scanning electronic micrographs
Wang Q, Mynar JL, Yoshida M, Lee E, Lee M, Okuro K, Kinbara K, Aida T (2010) High-water-content mouldable hydrogels by mixing clay and a dendritic molecular binder. Nature 463:339–343
Zhou H, Jin X, Yan B, Li X, Yang W, Ma A, Zhang X, Li P, Ding X, Chen W (2017) Mechanically Robust, Tough, and Self-Recoverable Hydrogels with Molecularly Engineered Fully Flexible Crosslinking Structure. Macromol Mater Eng 302(9):1700085
Kopecek J (2002) Polymer chemistry: swell gels. Nature 417:388–389
Biswas S, Rasale DB, Das AK (2016) Blue light emitting self-healable graphene quantum dot embedded hydrogels. RSC Adv 6:54793–54800
Rose S, Prevoteau A, Elziere P, Hourdet D, Marcellan A, Leibler L (2013) Nanoparticle solutions as adhesives for gels and biological tissues. Nature 505:382–385
Kim S, Jeon H, Shin S, Park S, Jegal J, Hwang S, Oh D, Park J (2018) Superior Toughness and Fast Self-Healing at Room Temperature Engineered by Transparent Elastomers. Adv Mater 30:1705145
Ihsan AB, Sun TL, Kurokawa T, Karobi SN, Nakajima T, Nonoyama T, Roy CK, Luo F, Gong JP (2016) Self-Healing Behaviors of Tough Polyampholyte Hydrogels. Macromolecules 49:4245–4252
Guo S, Dipietro LA (2010) Factors Affecting Wound Healing. J Dent Res 89:219–229
Yanagisawa Y, Nan Y, Okuro K, Aida T (2018) Mechanically robust, readily repairable polymers via tailored non-covalent cross-linking. Science 359:72–76
Truby RL, Lewis JA (2016) Printing soft matter in three dimensions. Nature 540:371–378
Sun JY, Zhao X, Illeperuma WRK, Chaudhuri O, Oh KH, Mooney DJ, Vlassak JJ, Suo Z (2012) Highly stretchable and tough hydrogels. Nature 489:133–136
Yu F, Cao X, Du J, Wang G, Chen X (2015) A Multi-Functional Hydrogel with Good Structure Integrity, Self-healing and Tissue-adhesive Property Formed by Combining Diels-Alder Click Reaction and Acylhydrazone Bond. ACS Appl Mater Inter 7:24023–24031
Han D, Yan L (2014) Supramolecular hydrogel of chitosan in the presence of graphene oxide Nanosheets as 2D cross-linkers. ACS Sustain Chem Eng 2:296–300
Zhang HJ, Xia HS, Zhao Y (2012) Poly(vinyl alcohol) hydrogel can autonomously self-heal. ACS Macro Lett 1:1233–1236
Tao F, Qin LM, Wang ZK, Pan QM (2017) Self-healable and cold-resistant supercapacitor based on a multifunctional hydrogel electrolyte. ACS Appl Mater Inter 9:15541–15548
Jing L, Li H, Tay RY, Sun B, Tsang SH, Cometto O, Lin J, Teo EHT, Tok AIY (2017) Biocompatible hydroxylated boron nitride Nanosheets/poly(vinyl alcohol) interpenetrating hydrogels with enhanced mechanical and thermal responses. ACS Nano 11:3742–3751
Zhang L, Wang Z, Xu C, Li Y, Gao J, Wang W, Liu Y (2011) High strength graphene oxide/polyvinyl alcohol composite hydrogels. J Mater Chem 21:10399–10406
Wang M, Nudelman F, Matthes RR, Shaver MP (2017) Frustrated Lewis pair polymers as responsive self-healing gels. J Am Chem Soc 139:14232–14236
Wu J, Cai L, Weitz DA (2017) Tough self-healing elastomers by molecular enforced integration of covalent and reversible networks. Adv Mater 29:1702616
Si Y, Wang L, Wang X, Tang N, Yu J, Ding B (2017) Ultrahigh-water-content, superelastic, and shape-memory nanofiber-assembled hydrogels exhibiting pressure-responsive conductivity. Adv Mater 29:1700339
Duan ZQ, Liu YT, Xie XM, Ye XY (2013) A simple and green route to transparent boron nitride/PVA nanocomposites with significantly improved mechanical and thermal properties. Chinese Chem Lett 24:17–19
Gao GR, Du GL, Sun Y, Fu J (2015) Self-healable, tough, and ultrastretchable nanocomposite hydrogels based on reversible polyacrylamide/montmorillonite adsorption. ACS Appl Mater Inter 7:5029–5507
Zhong M, Liu YT, Xie XM (2015) Self-healable, super tough graphene oxide/poly(acrylic acid) nanocomposite hydrogels facilitated by dual cross-linking effects through dynamic ionic interactions. J Mater Chem B 3:4001–4008
Lei WW, Mochalin VN, Liu D, Qin S, Gogotsi Y, Chen Y (2015) Boron nitride colloidal solutions, ultralight aerogels and freestanding membranes through one-step exfoliation and functionalization. Nat Commun 6:8849
Liu D, Lei WW, Qin S, Klika KD, Chen Y (2016) Superior adsorption of pharmaceutical molecules by highly porous BN nanosheets. Phys Chem Chem Phys 18:84–88
Wu YP, Xue Y, Qin S, Li J, Wang X, Bando Y, Golberg D, Chen Y, Gogotsi Y, Lei WW (2017) BN Nanosheet/polymer films with highly anisotropic thermal conductivity for thermal management applications. ACS Appl Mater Inter 9:43163–43170
Wu YP, Xue Y, Qin S, Liu D, Lei WW (2018) Super-compatible functional boron nitride nanosheets/polymer films with excellent mechanical properties and ultra-high thermal conductivity for thermal management. J Mater Chem C 6:1363–1369
Wu YP, Guo ML, Liu GF, Xue SS, Xia YM, Liu D, Lei WW (2018) Surface modification of boron nitride nanosheets by polyelectrolytes via atom transfer radical polymerization. Mater Res Express 5(4):045026 doi.org/10.1088/2053-1591/aab8ec
Yan XZ, Liu ZY, Zhang QH, Lopez J, Wang H, Wu HC, Niu SM, Yan HP, Wang SH, Lei T, Li JH, Qi DP, Huang PG, Huang JP, Zhang Y, Wang YY, Li GL, Tok JBH, Chen XD, Bao ZN (2018) Quadruple H-bonding cross-linked supramolecular polymeric materials as substrates for stretchable, Antitearing, and self-healable thin film electrodes. J Am Chem Soc 140:5280–5289
Cong HP, Wang P, Yu SH (2014) Highly Elastic and Superstretchable Graphene Oxide/Polyacrylamide Hydrogels. Small 10:448–453
Cui W, Ji J, Cai YF, Li H, Ran R (2015) Robust, anti-fatigue, and self-healing graphene oxide/hydrophobic association composite hydrogels and their use as recyclable adsorbents for dye wastewater treatment. J Mater Chem A 3:17445–17458
Zhao L, Huang J, Zhang Y, Wang T, Sun W, Tong Z (2017) Programmable and bidirectional bending of soft actuators based on Janus structure with sticky tough PAA-clay hydrogel. ACS Appl Mater Inter 9:11866–11873
Rahimi N, Molin DG, Cleji TJ, Zandvoort MA, Post MJ (2012) Electrosensitive polyacrylic acid/fibrin hydrogel facilitates cell seeding and alignment. Biomacromolecules 13:1448–1457
Jiang H, Wang Z, Geng H, Song X, Zeng H, Zhi C (2017) Highly Flexible and Self-Healable Thermal Interface Material Based on Boron Nitride Nanosheets and a Dual Cross-Linked Hydrogel. ACS Appl Mater Inter 9:10078
Hu X, Liu J, He Q, Meng Y, Cao L, Sun Y, Chen J, Lu F (2016) Aqueous compatible boron nitride nanosheets for high-performance hydrogels. Nanoscale 8:4260–4266
Pan C, Liu L, Chen Q, Zhang Q, Guo G (2017) Tough, stretchable, compressive novel polymer/graphene oxide nanocomposite hydrogels with excellent self-healing performance. ACS Appl Mater Inter 9:38052–38061
Darabi MA, Khosrozadeh A, Mbeleck R, Liu Y, Chang Q, Jiang J, Cai J, Wang Q, Luo G, Xing M (2017) Skin-inspired multifunctional autonomic-intrinsic conductive self-healing hydrogels with pressure sensitivity, Stretchability, and 3D printability. Adv Mater 29:1700533
Das S, Irin F, Ma L, Bhattacharia SK, Hedden RC, Green MJ (2013) Rheology and Morphology of Pristine Graphene/Polyacrylamide Gels. ACS Appl Mater Inter 5:8633–8640
Cong HP, Wang P, Yu SH (2013) Stretchable and Self-Healing Graphene Oxide–Polymer Composite Hydrogels: A Dual-Network Design. Chem Mater 25:3357–3362
Xiong L, Hu X, Liu X, Tong Z (2008) Network chain density and relaxation of in situ synthesized polyacrylamide/hectorite clay nanocomposite hydrogels with ultrahigh tensibility. Polymer 49:5064–5071
Tang Z, Chen F, Chen Q, Zhu L, Yan X, Chen H, Ren B, Yang J, Qin G, Zheng J (2017) Energy Dissipation and Mullins Effect of Tough Polymer/Graphene Oxide Hybrid Nanocomposite Hydrogels. Polym Chem 8:4659–4672
Cui ZH, Martinez AP, Adamson DH (2015) PMMA functionalized boron nitride sheets as nanofillers. Nanoscale 7:10193–10197
Li J, Illeperuma WRK, Suo Z, Vlassak JJ (2014) Hybrid hydrogels with extremely high stiffness and toughness. ACS Macro Lett 3:520–523
This work was financially supported by Foundation of Sichuan Youth Science and Technology (2016JQ0036), Fok Ying Tung Education Foundation (161103), Open Funds of State Key Laboratory of Petroleum Pollution Control (PPC2017008) and State Key Laboratory Oil and Gas Reservoir Geology and Exploitation (PLN1201, SWPU), Natural Science Foundation of Nanchong City (NC17SY4015), and Innovative Research Team of Southwest Petroleum University (2017CXTD01).
Foundation of Sichuan Youth Science and Technology (2016JQ0036).
Fok Ying Tung Education Foundation (161103).
Open Funds of State Key Laboratory of Petroleum Pollution Control (PPC2017008) and State Key Laboratory Oil and Gas Reservoir Geology and Exploitation (PLN1201, SWPU).
Natural Science Foundation of Nanchong City (NC17SY4015).
Training Program of Innovation and Entrepreneurship for Undergraduates (201710615006).
Innovative Research Team of Southwest Petroleum University (2017CXTD01).
Availability of Data and Materials
The datasets supporting the conclusions of this article are available in the [repository name] repository [unique persistent identifier and hyperlink to datasets in http:// format].
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Figure S1. Tensile stress-strain curves of B0Py hydrogels with different water contents. Figure S2. Tensile stress-strain curves of B0.1Py hydrogels with different water contents. Figure S3. Tensile stress-strain curves of B0.5Py hydrogels with different water contents. Figure S4. Tensile stress-strain curves of B0.8Py hydrogels with different water contents. Figure S5. Tensile stress-strain curves of B1.0Py hydrogels with different water contents. Figure S6. The digital photograph of torsion hydrogel. Figure S7. Young’s modulus of hydrogels of BxP50 and BxP70. Figure S8. the fracture stresses of original BxP25 hydrogels and healed BxP25 hydrogels with different BNNS-NH2 concentrations (the healing time was 1 h). (DOCX 783 kb)